converters for steel production was gradually, partially replaced by the electric arc furnace using scrap steel and iron. In Japan the share of LD process decreased from 80% in 1970 to 70% in 2000; worldwide share of the basic oxygen process stabilized at 60%. Process Basic oxygen steelmaking is a primary steelmaking process for converting molten pig iron into steel by blowing oxygen through a lance over the molten pig iron inside the converter. Exothermic heat is generated by the oxidation reactions during blowing. The basic oxygen steel-making process is as follows: Molten pig iron (sometimes referred to as "hot metal") from a blast furnace is poured into a large refractory-lined container called a ladle. The metal in the ladle is sent directly for basic oxygen steelmaking or to a pretreatment stage. Pretreatment of the blast furnace hot metal is done externally to reduce sulfur, silicon, and phosphorus before charging the hot metal into the converter. In external desulfurising pretreatment, a lance is lowered into the molten iron in the ladle and several hundred kilograms of powdered magnesium are added and the sulfur impurities are reduced to magnesium sulfide in a violent exothermic reaction. The sulfide is then raked off. Similar pretreatments are possible for external desiliconisation and external dephosphorisation using mill scale (iron oxide) and lime as fluxes. The decision to pretreat depends on the quality of the hot metal and the required final quality of the steel. Filling the furnace with the ingredients is called charging. The BOS process is autogenous, i.e. the required thermal energy is produced during the oxidation process. Maintaining the proper charge balance, the ratio of hot metal from melt to cold scrap is important. The BOS vessel can be tilted up to 360° and is tilted towards the deslagging side for charging scrap and hot metal. The BOS vessel is charged with steel or iron scrap (25–30%),if required. Molten iron from the ladle is added as required for the charge balance. A typical chemistry of hotmetal charged into the BOS vessel is: 4% C, 0.2–0.8% Si, 0.08%–0.18% P, and 0.01–0.04% S, all of which can be oxidised by the supplied oxygen except sulfur (which requires reducing conditions). The vessel is then set upright and a water-cooled, copper tipped lance with 3–7 nozzles is lowered into it to within a few feet of the surface of the bath and high-purity oxygen at a pressure